To evaluate the durability of dentin bonding over time, the nanoleakage of four dentin bonding systems (Single Bond, Stae, Clearfil SE Bond and PermaQuik) over 24 hours, three months, six months and 12 months, was investigated. Flat occlusal dentin surfaces from extracted human molars were finished with wet 600-grit silicon carbide paper and bonded with one of the dentin bonding systems following manufacturers' instructions. The bonded surface was covered with < 1 mm thick layer of Silux Plus resin composite and light cured for 40 seconds. The specimens in each dentin-bonding group were randomly assigned to four sub-groups and kept in phosphate buffered saline solution (pH 7.4) containing 0.01% sodium azide at 37 degrees C for 24 hours, three, six or 12 months. The margins of all specimens were finished and polished with Sof-Lex disks after initial 24-hour storage. At the end of each storage time, the surrounding tooth surfaces except for 1 mm adjacent to the restoration were coated with nail varnish. The samples were immersed in a 50% w/v solution of silver nitrate for 24 hours, placed in photodeveloping solution and exposed to fluorescent light for eight hours. The samples were cut longitudinally and buccoligually, polished, mounted on stubs, carbon coated and observed in a Field Emission-SEM using backscattered electron mode. The results showed that systems using phosphoric acid as the etchant had a line of silver deposition at the base of the hybrid layer. Silver deposition increased in all systems over 12-months storage, with PermaQuik changing the least. Nanoleakage of the dentin bonding systems increased slightly during the 12-month storage period, indicating that they may be subject to hydrolytic attack over time.